A transparent coating that repels a wide variety of liquids, prevents staining, is capable of self-repair and is robust towards mechanical damage can have a broad technological impact, from solar cell coatings to self-cleaning optical devices. Here we employ colloidal templating to design transparent, nanoporous surface structures. A lubricant can be firmly locked into the structures and, owing to its fluidic nature, forms a defect-free, self-healing interface that eliminates the pinning of a second liquid applied to its surface, leading to efficient liquid repellency, prevention of adsorption of liquid-borne contaminants, and reduction of ice adhesion strength. We further show how this method can be applied to locally pattern the repellent character of the substrate, thus opening opportunities to spatially confine any simple or complex fluids. The coating is highly defect-tolerant due to its interconnected, honeycomb wall structure, and repellency prevails after the application of strong shear forces and mechanical damage. The regularity of the coating allows us to understand and predict the stability or failure of repellency as a function of lubricant layer thickness and defect distribution based on a simple geometric model.
Motivated by a broad potential impact on science and technology, the design of liquid-repellent surfaces has been the subject of intense research that has led to the development of superhydrophobic1,2,3,4 and, more recently, superomniphobic5,6,7,8,9 surface coatings, which show resistance to water and organic liquids, respectively. The design of such surfaces has been adapted from nature’s famously self-cleaning lotus leaves10. The underlying design principle is the reduction of contact points of a liquid droplet by the introduction of roughness features. Thus, a solid/air composite surface is created11 that enables liquid droplets to roll off with ease. Despite remarkable improvements in liquid repellency5,6,7,8, transparency7,12 and durability7,13 made possible by increasingly sophisticated surface microstructure designs, several challenges remain: most importantly, the adsorption of proteins or bacteria to superhydrophobic surfaces14,15, pressure instability16,17, limited self-healing properties and the impossibility of creating thermodynamically stable non-wetting states for low-surface-tension liquids6.
The development of lubricant-infused porous materials, inspired by nature’s Nepenthes pitcher plant18, has recently introduced a new paradigm for the creation of surfaces with the capability to repel arbitrary aqueous and organic liquids19. In contrast to the lotus-inspired approach, these slippery liquid-infused porous surfaces (SLIPS) are designed to create a fluid/fluid interface between a lubricant and the immiscible liquid to be repelled. To maintain stable repellency, such a surface needs to be optimized in a way that the lubricant layer is not displaced from the solid’s surface: if the free energy of the solid/lubricant/liquid system is minimal for the situation where the test liquid resides on the lubricant layer without replacing it, the liquid/liquid interface effectively eliminates pinning points, leading to super-repellent surfaces with extremely low sliding angles—even for liquids with very low surface tensions. Additionally, the fluid nature of the interface possesses self-healing characteristics, allows for remarkable pressure-stability19 and has been shown to effectively prevent the attachment of bacteria20 and ice21, thus overcoming many of the challenges of conventional repellent surfaces.
Though conceptually different, both lotus-inspired and SLIPS designs require roughness to support repellency. For a SLIPS surface, this roughness—paired with surface functionalization to match the chemical nature of the lubricant—allows effective confinement of the lubricant inside the structured solid. In initial attempts, perfluorinated lubricants were wicked into porous Teflon membranes that provided both matching fluorinated surface functionalities as well as a nanoporous confinement.19 Additionally, chemically functionalized micron-scale roughness features prepared by conventional and soft lithography19,20,22,23, electrodeposition of polypyrrole nanostructures21 and sol-gel derived aluminium oxide nanostructures24,25 have recently been successfully employed as structured solids for lubricant infiltration.
Here we report on the design of a fully transparent SLIPS coating based on colloidal templating26,27,28,29. In our approach, a colloidal monolayer is backfilled by a silica precursor to form an inverse replica that serves as a porous layer to lock-in the lubricant. There are multiple reasons to employ colloids as building blocks. The regular arrangement of colloids in a monolayer30 is experimentally simple, fast and cheap and gives access to nanopores of well-defined size, shape and order, thus allowing us to precisely calculate and control surface roughness. In contrast to irregular nanostructures, this enables a fundamental analysis of the stability of a liquid-infused coating based on geometric models. The silica backfilling allows for strong, covalent bonding of the nanostructured film to glass or oxide substrates, preventing delamination or adhesive failure of the film and thus enhancing the robustness of the surface structures. Additionally, it can be modified by well-developed silane chemistry that provides a broad range of stable, covalently bound monolayers terminated with surface functionalities matched to the properties of the lubricant. The tunability of pore sizes at the nanometre scale can be used to engineer the optical properties of materials across a wide range of wavelengths and enables the formation of transparent surface coatings12, a prerequisite, for example, for the application of SLIPS to windows or solar cells. Homogeneity and chemical resistance of the colloid-templated silica coating allows for the application of conventional photolithography to pattern the repellent character of the surface. The combination of the strong liquid repellency of a SLIPS coating with surface patterning protocols is of high practical interest as it may open pathways to confine low-surface-tension liquids (for example, oil) and complex fluids (for example, blood) to designated parts of a surface. This novel methodology could be implemented to create SLIPS-based microfluidic devices that operate without solid interfaces or could be used to confine small blood droplets into microscopic arrays, for example, for medical diagnostics31,32.
Surface structure design and liquid repellency
The key challenge in designing highly repellent lubricant-infused structured surfaces by colloidal templating is the ability to homogeneously cover large areas of solid substrates with colloidal monolayers. In our approach, we preassemble colloids at the air/water interface and subsequently transfer them to the desired substrates33,34. The liquid nature of the interface provides fluidity necessary to achieve high order and uniform coverage and inherently confines the colloids to a two-dimensional layer. This avoids the formation of multilayers that might act as pinning points for applied test liquids and compromise repellency. Additionally, the process allows for uniformly depositing colloidal monolayers over large areas, limited only by the dimensions of the water’s surface, and is able to cover curved or topographically structured surfaces33,34,35.
Figure 1a schematically shows the construction of a SLIPS coating from a colloidal template. Structural details and the high uniformity and regularity of the prepared nanoporous layer can be seen in SEM images (Fig. 1h and Supplementary Fig. S1). Figure 1b–g compares the wetting properties of the nanostructured surfaces made from 1 μm colloids in dry and lubricated states. The dry, fluorinated structures show superhydrophobic characteristics27 with high dynamic contact angles and reasonably low sliding angles (Fig. 1b). However, they fail to repel low-surface-tension octane: a withdrawing droplet is strongly pinned to the surface, leading to an extremely high contact angle hysteresis, and will not slide off the substrate even when placed vertically (Fig. 1c). When the same substrate is infused with a fluorinated lubricant, drastic changes are observed: the complete elimination of pinning points induces super-repellency with high droplet mobility that leads to extremely low sliding angles for both water and octane (Fig. 1d,e). A quantitative assessment of contact angle hysteresis and minimum sliding angles (5 μl droplet) for liquids with a range of surface tensions (water, ethylene glycol and octane) shown in Fig. 1f,g further highlights the significant differences between the dry and lubricated states and reveals the highly efficient repellency of the SLIPS coating compared to its superhydrophobic analogue. It is noteworthy that the repellent properties of these surfaces are not limited to the use of fluorinated liquids as lubricants: with a proper adjustment of the surface chemistry, a variety of different fluids can be used as lubricants to repel a second, immiscible liquid. As examples, we show the water-repellent properties of hexadecane- and olive oil-infused coatings functionalized with hydrophobic decyltrichlorosilane molecules or, more remarkably, the repellency of the fluorinated oil itself by water-infused hydrophilic inverse monolayers (Supplementary Fig. S2, Supplementary Movie 1).
The pore size of the inverse monolayers was adjusted from 140 to 1,060 nm by changing the colloid size while maintaining close-packed order and regularity (Fig. 2a). Downscaling the structure sizes has strong effects on the optical properties. Figure 2b compares UV-Vis-NIR transmission spectra of the differently sized inverse monolayers deposited on one side of microscope slides at normal incidence in dry (black lines) and lubricated states (red lines), and to untreated glass slides (dotted black lines). The large colloids (1,060 nm) show a strong coloration arising from Mie resonances of the individual structures and diffractively coupled resonances of the ordered structures36. With decreasing feature size, light losses are strongly diminished and the substrate’s transparency is identical to a plain glass slide used as a control. The addition of the lubricant decreases the refractive index contrast, leading to a drastic reduction in light losses. From a colloid template size of 415 nm, no loss of transmitted light intensity is detected and the substrates appear as transparent as regular glass slides. For colloid template sizes of 225 nm and 138 nm, the SLIPS coating leads to enhanced light transmission of up to 3%. We attribute the enhanced transmission to the reduced refractive index contrast of the lubricant/air interface compared to the original glass/air interface.
The influence of the feature size of the surface structure on the liquid repellency was assessed by measurements of the minimum sliding angle of octane in dry and lubricated states (Fig. 2c) and the corresponding contact angle hysteresis (Supplementary Fig. S3). A strong difference in wetting characteristics can be seen for all colloid template sizes. Dry samples show pinning of the droplet and high contact angle hysteresis. After lubrication all structure sizes support high repellency, with contact angle hysteresis and sliding angles not exceeding 5°. The SLIPS state is maintained for all colloid template sizes with all liquids tested (Fig. 2d). It is noteworthy that although the size of the pores does not affect the SLIPS characteristics, reference measurements performed on lubricated, fluorinated, flat samples without surface nanostructures show higher contact angle hysteresis and sliding angles, thus suggesting that the presence of the underlying surface roughness is required for efficient repellency.
We further demonstrate that transparent slippery coatings based on inverse colloidal monolayers can be easily applied to curved substrates, thus providing a self-cleaning coating for optical windows. Figure 2e shows time-lapsed images (taken from Supplementary Movie 2) of a watch glass covered with an inverse monolayer-based SLIPS coating that repels dyed octane droplets. Likewise, the curved surface of a glass vial was rendered slippery and showed perfect non-wetting behavior when immersed in dyed octane or water solutions (Supplementary Fig. S4 and Supplementary Movie 3).
In general, a major source of surface contamination arises from adsorption of liquid-borne contaminants to a solid surface in contact with the liquid. Such contamination not only stains common surfaces in every-day life but, when proteins or bacteria are present in the liquid, imposes severe threats to public health by seeding the formation of biofilms, a major source of infections in hospitals20,37,38. Moreover, the adsorption of matter from liquids onto the surface can change the surface chemistry and lead to a degradation of tailored surface properties, for example, its superhydrophobicity15,39. If direct contact of the liquid to the substrate is avoided, adsorption of contaminants to its surface can be prevented. We demonstrate that lubricated inverse monolayer substrates extremely reduce the adsorption of a variety of liquid-borne contaminants, caused by the absence of contact points between the contaminated liquid and the solid surface due to the presence of the lubricant layer, which provides a slippery, defect-free liquid/liquid interface. Figure 3a–c presents fluorescence microscopy images of fluorinated, superhydrophobic inverse-monolayer surfaces without (upper row) and with (lower row) lubricant after exposure to dyed water (a), octane (b) and undiluted fetal bovine serum (c). All superhydrophobic samples failed to prevent adhesion: even though they feature high water repellency, a direct contact between the liquid and the solid cannot be avoided, leading to a rapid adsorption of liquid-borne contaminants to the hydrophobic surface14. In comparison, the lubricated, SLIPS samples showed negligible contamination. We envision the resistance of this transparent surface coating to protein adhesion will have a strong impact on the design of non-fouling optical windows in biomedical devices, but focus here on simple consumer applications by demonstrating the effective repellency and complete absence of staining of SLIPS-modified glass slides after spilling of red wine, olive oil and ketchup (Fig. 3d–f, Supplementary Movie 4).
The strong adhesion of ice to most common surfaces, causing safety and economic issues in any technology subjected to sub-zero environments, is another example where the direct contact of the material with the substrate is the principal cause for its detrimental effects. We recently demonstrated that SLIPS coatings based on highly textured polypyrrole drastically lower strength of ice adhesion to aluminium substrates21. Of further importance is the ability to impart transparency to such ice-repellent coatings. Figure 3g compares the adhesion strength of ice (measured at −40 °C using a custom ice adhesion setup adapted from literature)21,40 for different glass substrates. The strong adhesion of ice to hydrophilic glass (1318±63 kPa) decreases with fluorination of the surface but is still substantial (743±334 kPa). The presence of a superhydrophobic, fluorinated inverse monolayer structure further decreases the ice adhesion strength (387±204 kPa). The addition of a lubricant to form a SLIPS coating drastically reduces the adhesion of ice by more than one order of magnitude compared to the superhydrophobic substrate (by decoupling the ice formation from the solid substrate). The measured ice adhesion strength on the transparent SLIPS coating (10±7 kPa) is in excellent agreement with our previous results on SLIPS coatings on aluminium21, suggesting that the surface properties are governed by the lubricant layer and not the solid substrate itself.
Patterned wetting properties
The uniformity and low height of the structures enables the application of conventional photolithographic processes to prepare locally confined patterned SLIPS regions (Fig. 4a). The process is based on the creation of surface functionality patterns. The lubricant is only locked-in firmly in areas with matching surface chemistry, while it will be replaced by a second liquid in areas with different surface chemistry. However, due to its low surface energy, addition of the lubricant leads to a homogeneous lubricant film covering the entire coating. Upon addition of a second liquid, a metastable state can be created in which the lubricant layer is not immediately disrupted by the applied liquid (Fig. 4a). Eventually, the energetically most favourable state is reached as the liquid displaces the lubricant layer in non-functionalized surface regions. Stable SLIPS surface regions defined by the fluorinated surface chemistry remain wetted solely by the lubricant.
The superior performance of the SLIPS-based approach to create patterns of liquids on solid substrates is revealed in Fig. 4b–d and in Supplementary Movies 5 and 6. The figure shows the successful confinement of several test liquids to designated surface regions based on matching surface chemistry. Owing to its high surface tension, water can be confined to hydrophilic surface regions on a dry, patterned substrate as well as with the SLIPS-based approach (Fig. 4b). An advantage of the latter is the prevention of adhesion of contaminants from the water phase that cannot be excluded for the dry patterning approach (compare to Fig. 3). Octane, as a low-surface-tension test liquid (Fig. 4c), and sheep blood, as an example of a complex fluid (Fig. 4d), fail to be confined on the dry, patterned substrate: both liquids wet the entire surface, whereas a clear pattern can be resolved in the SLIPS-based approach. The creation of patterns of such fluids is extremely challenging with state-of-the-art coatings.
Assessment of thermodynamic stability and defect tolerance
Compared to existing approaches to creating nanoscale surface patterns19,21,24, the design of SLIPS coatings using a simple, bottom-up colloidal self-assembly process produces surface structures with finely controlled feature sizes, high regularity and uniformity. This allows us to analyze and compare the stability of the transparent SLIPS coatings with theoretical predictions based on thermodynamic considerations, and thus advance the fundamental understanding of the surface properties and function. We start by calculating the minimum surface roughness R—defined as the ratio of the surface area of the porous substrate to that of a flat surface—required to support a stable SLIPS condition based on the surface energy balance concept19,23. The stability of a system with a droplet of liquid A (contact angle θA, surface tension γA) sitting on top of a film of lubricant B (θB, γB; interfacial tension of the two liquids γAB) is predicted by19:
For octane as droplet and DuPont Krytox 100 as lubricant, we yield R >1.51±0.1 as the threshold value to support stable SLIPS (Supplementary Note 1). A geometric analysis of the inverse monolayer structure estimates the roughness factor to be 1.91 (Supplementary Note 1). Hence, a uniform inverse colloidal monolayer is indeed capable of supporting a thermodynamically stable configuration. Additionally, it is worth noting that SLIPS stability, as predicted by the equation, is not a function of the actual structure size, thus providing the thermodynamic foundation for the design of completely transparent coatings based on increasingly small feature sizes.
In applications, it is critical to understand the defect tolerance and the associated thermodynamic penalties of imperfect or damaged SLIPS coatings. The inverse monolayer substrates provide a perfect system to assess these parameters. By varying the amount of tetraethylorthosilicate (TEOS) used for the inverse monolayer preparation, it is possible to tune the surface coverage of the nanostructures from an intact inverse monolayer to highly damaged surfaces featuring only small monolayer patches (Fig. 5a, Supplementary Fig. S5). The length scale of the defects on the substrates is on the order of few micrometres (Supplementary Fig. S6) and, hence, small compared to the dimension of a macroscopic liquid droplet. Thus, the droplet experiences a total roughness that is averaged from intact inverse monolayer and monolayer-free areas. We systematically adjusted the total roughness of surfaces from 1.0 (flat, unstructured glass surface) to 1.91 (intact structure) and, after fluorosilanization and addition of a lubricant, investigated their performance in repelling octane (Fig. 5d). All structured samples show effective octane repellency, as indicated by very small sliding angles (<5°). Comparing the roughness values in the experiment with the calculated minimum surface roughness, we conclude that the more damaged samples support a metastable SLIPS coating that, even though not in its thermodynamically stable state, sustain their repellent character, at least over the time frame of the experiment and in the absence of any external stresses. Placement of an octane droplet onto the substrates over a longer time (>15 min) revealed pinning for the most damaged sample (R=1.14), while all other substrates remained repellent, corroborating metastability of the coating in short-term applications. We further note that while the thermodynamic calculations are derived from the four-phase substrate/lubricant/liquid/air system, a more fundamental requirement for SLIPS is the ability of the lubricant to wet the surface homogeneously (that is, apparent contact angle θ*=0°). Using Wenzel’s relation (cosθ*=R cosθ) 41, we calculate the minimum roughness needed for complete wetting to be 1.11 (θKrytox=26.1°). Thus, we attribute the unexpected repellent behavior of highly damaged samples to their ability to support homogeneous wetting of the lubricant, the replacement of which by the probe liquid is slow compared to the experimental time frame. By virtue of the same argument, the flat sample fails to support high repellency because it is not completely wetted by the lubricant and thus exposes dry, de-wetted areas to which the octane droplet adheres (Fig. 5d, insets).
The substrates were also subjected to high shear forces induced by spin-coating at increasing rotational speeds (Fig. 5b). Figure 5e shows the resulting octane sliding angles after the final step of spin-coating at 10,000 r.p.m. Remarkably, substrates with a roughness of >1.61 did not lose their repellency and showed low sliding angles <5°, implying the presence of an intact lubricant layer completely covering the porous solid (Fig. 5e, insets 1–2). All other samples showed increased sliding angles, indicating partial loss of the lubricant layer at the damaged parts of the substrate and subsequent pinning of octane at the exposed solid surface (Fig. 5e, insets 3, 4). To demonstrate the superior performance of the presented coating, an open-cell epoxy micropillar sample19 was subjected to the same spin-coating protocol and failed to retain its repellency after 2,000 r.p.m. (Supplementary Fig. S7). We established a simple model to predict the onset of lubricant de-wetting caused by a defect between regular surface structures (Fig. 5c). The model correlates the critical defect length lcrit (the maximum defect length that supports complete lubricant coverage) with the thickness h and the contact angle of the lubricant on the solid substrate (Supplementary Note 2, Supplementary Figures S8–S11):
Figure 5f compares the experimentally measured lubricant layer thicknesses after the individual spin-coating steps (data points) to the calculated critical lubricant thicknesses (solid lines). Once the measured thickness drops below the theoretically calculated value, de-wetting and hence failure to repel octane is expected. A comparison between the predicted and measured repellency failures yielded an excellent agreement (Table 1). Thus, our simple model accurately explains and predicts stable repellency or failure for any given damaged sample at all different spinning speeds.
The experiments reveal a remarkable affinity of the lubricant layer to the porous surface. Samples with a substantial amount of damage (up to 33% of the complete surface) continuously support repellency even at the maximum rotational speeds available in our setup. This has important consequences for creating robust coatings for industrial and consumer applications. We further note that our thermodynamically stable coatings maintain their repellency over an extended period of time, which we confirmed by the long-term stability of octane repellency on vertically stored substrates, mimicking an actual window (Fig. 6a). Even after >9 months of vertical storage without replenishment of lubricant, all samples continue to show octane sliding angles well below 10°. Moreover, the closed-cell architecture of the inverse monolayer paired with the efficient, covalent binding of the silica sol–gel on glass adds superior mechanical stability to the nanoscale coating. Figure 6b demonstrates the complete structural integrity of inverse monolayer samples after being subjected to a variety of mechanical treatments including touching, wiping and tape peel tests. An open-cell reference sample consisting of epoxy micropillars was completely destroyed by any of the treatments (Fig. 6b, insets). The combination of high mechanical stability of the structures (Fig. 6b), damage tolerance of the lubricant-infused coating (Fig. 5b) and the unique self-healing properties arising from the liquid nature of the lubricant19 suggests that the surfaces can tolerate various mechanical treatments likely to occur in daily-life applications. In Fig. 6c–e, we present still frames taken from Supplementary Movie 7 demonstrating the retention of high repellency after mechanical damage induced by cleaning with a tissue (c), scratching with a razor blade (d) and treatment with sandpaper (e).
We conclude by briefly discussing the characteristic properties of the lubricant-infused inverse monolayer-based coating. The surfaces combine all the attractive properties of previously reported SLIPS coatings, including highly effective liquid repellency toward a variety of liquids, prevention of contamination and a strong decrease of ice adhesion strength. The process can be scaled and allows coating of curved substrates. The size of the pores can be tuned over a wide range, and can be designed to be small enough to not interfere with light of visible wavelengths and even to enhance the transmission of light, leading to omniphobic, optically clear coatings required in many applications where transparency of the surface is critical. The coating exhibits remarkably robust surface structures, resulting from the interconnected pore geometry of the inverse monolayer paired with the stable, covalent adhesion of the silica scaffold to oxide surfaces. Its repellent character is retained after extended periods of time and repellency prevails after the application of strong shear forces and mechanical damage. The methodology is compatible with conventional patterning processes, which can be used to create locally confined SLIPS patterns on a substrate, allowing confinement of low-surface-tension liquids and complex fluids to designated surface areas.
In addition to the demonstrated performance characteristics of these surfaces, their high uniformity and order coupled with the ability to regulate the defect distribution allow for precise control of the surface roughness and comparison of the stability of the SLIPS coating with theoretical predictions, leading to a deeper insight into the mechanisms of wetting occurring on SLIPS surfaces. We show that the lubricant-infused inverse monolayers are thermodynamically stable for intact structures while heavily damaged structures can support a metastable repellency state. Furthermore, we develop a simple geometric model that can be applied to predict the stability or failure of the coating as a function of the lubricant layer thickness and the size of defects in the samples.
All these characteristics add to a versatile surface coating with an unprecedented combination of properties. A wide variety of applications of the presented technology can be envisioned, including omniphobic, self-cleaning and self-healing windows or solar panels, face shields, glasses, goggles or lenses and non-fouling windows or surface patterns in biomedical diagnostic assays or devices.
Formation of colloidal monolayers on glass
Colloidal monolayers were crystallized on the air–water interface of a crystallization dish following a protocol from literature34. Briefly, a colloidal dispersion in 1:1 water/ethanol (solid content ~2.5%) was spread onto the interface via a glass slide until the surface was completely covered. The substrate was then inserted into the subphase and the monolayer was deposited manually by fishing out the slide. After drying, a closed-packed monolayer uniformly covered the substrate. All colloids were prepared by surfactant-free emulsion polymerization of styrene with acrylic acid as comonomer.
Formation of the inverse monolayer
A solution of tetraethylorthosilicate (TEOS), HCl (0.1 mol l−1) and ethanol with weight ratios of 1:1:1.5 was prepared and stirred for 1 h. Then, it was diluted with ethanol (for dilution ratios, see Supplementary Table S1) and spin-coated onto the monolayer-covered substrate (3,000 r.p.m., 30 s, acceleration 500). The colloids were removed by combustion at 500 °C (ramped from RT to 500 °C for 5 h, 2 h at 500 °C). To prepare damaged surfaces, the TEOS concentration was systematically decreased as specified in Supplementary Table S2.
Fluorosilanization was carried out by vapor-phase deposition of (1H,1H,2H,2H-tridecafluorooctyl)-trichlorosilane (or Decyltrichlorosilane) for 24 h at reduced pressure and room temperature. Prior to silanization, the substrates were cleaned in acid piranha (3:1 sulphuric acid:hydrogen peroxide; warning: reacts very violently with organic materials) and plasma-treated with oxygen plasma for 10 min.
10 μl cm−2 Krytox 100 (or similar amounts of water or olive oil) was added to the substrate and uniform coverage was achieved by tilting. Excess lubricant can be removed by vertical placement of the substrates. For the long-term experiment, the more viscous Krytox 103 was used to minimize the evaporation of the lubricant.
A conventional photoresist (S1818, positive tone resist) was spin-coated (4,000 r.p.m., 60 s) on the unsilanized inverse monolayer substrate. Illumination with UV light was performed by following the recipe of the photoresist manufacturer (Shipley Company, Marlborough, MA) with an irradiation dose of 200 mJ cm−2 followed by development of the structures (Developer MF319, 60 s). The substrate, consisting of areas covered by photoresist and free areas was plasma-treated for 5 min and then fluorosilanized similar to non-patterned substrates. After silanization, the resist was washed off the substrate (Remover PG 1165). The application of a lubricant then produced patterned SLIPS surfaces, as the conditions for a stable SLIPS state is only fulfilled in the fluorosilane-functionalized surface regions.
The contact-angle measurements were performed with a contact-angle measurement system (KSV CAM 101) at room temperature with ~20% relative humidity. The droplet volume for the measurements was 5 μl (unless otherwise specified) and the macroscopic droplet profile was captured through a camera. The droplet profile was fitted into a spherical cap profile by a computer programme provided by the manufacturer of the system. Contact-angle hysteresis was measured by increasing and decreasing the droplet volume while taking screenshots and extracting the advancing and receding contact angles. Sliding angles were measured on a customized tilting stage with a droplet volume of 20 μl. All contact angle values specified in the text were averaged over at least 10 individual measurements.
Mechanical stability tests
The mechanical stability was assessed by (i) pressing a finger onto the surface structures, (ii) vigorously wiping it with an ethanol-soaked tissue, (iii) scratching with the razor-blade or sandpaper, and (iv) applying Scotch Tape to the coating followed by peeling off the tape. After the treatments, all surface structures were imaged by SEM.
How to cite this article: Vogel, N. et al. Transparency and damage tolerance of patternable omniphobic lubricated surfaces based on inverse colloidal monolayers. Nat. Commun. 4:2176 doi: 10.1038/ncomms3176 (2013).
Onda, T., Shibuichi, S., Satoh, N. & Tsujii, K. Super-water-repellent fractal surfaces. Langmuir 12, 2125–2127 (1996).
Feng, L. et al. Super-hydrophobic surfaces: from natural to artificial. Adv. Mater. 14, 1857–1860 (2002).
Patankar, N. A. Mimicking the lotus effect: Influence of double roughness structures and slender pillars. Langmuir 20, 8209–8213 (2004).
Nosonovsky, M. & Rohatgi, P. K. Biomimetics in Materials Science: Self-Healing, Self-Lubricating, and Self-Cleaning Materials. Springer (2012).
Tuteja, A. et al. Designing superoleophobic surfaces. Science 318, 1618–1622 (2007).
Tuteja, A., Choi, W., Mabry, J. M., McKinley, G. H. & Cohen, R. E. Robust omniphobic surfaces. Proc. Natl Acad. Sci. USA 105, 18200–18205 (2008).
Deng, X., Mammen, L., Butt, H. J. & Vollmer, D. Candle soot as a template for a transparent robust superamphiphobic coating. Science 335, 67–70 (2012).
Kota, A. K., Li, Y., Mabry, J. M. & Tuteja, A. Hierarchically structured superoleophobic surfaces with ultralow contact angle hysteresis. Adv. Mater. 24, 5838 (2012).
Hensel, R. et al. Wetting resistance at its topographical limit: the benefit of mushroom and serif T structures. Langmuir 29, 1100–1112 (2013).
Barthlott, W. & Neinhuis, C. Purity of the sacred lotus, or escape from contamination in biological surfaces. Planta 202, 1–8 (1997).
Cassie, A. B. D. & Baxter, S. Wettability of porous surfaces. Trans. Faraday Soc 40, 0546–0550 (1944).
Li, Y. et al. Biomimetic surfaces for high-performance optics. Adv. Mater. 21, 4731–4734 (2009).
Zhu, X. T. et al. Robust superhydrophobic surfaces with mechanical durability and easy repairability. J. Mater. Chem. 21, 15793–15797 (2011).
Sigal, G. B., Mrksich, M. & Whitesides, G. M. Effect of surface wettability on the adsorption of proteins and detergents. J. Am. Chem. Soc. 120, 3464–3473 (1998).
Mazumder, S., Falkinham, J. O., Dietrich, A. M. & Puri, I. K. Role of hydrophobicity in bacterial adherence to carbon nanostructures and biofilm formation. Biofouling 26, 333–339 (2010).
Poetes, R., Holtzmann, K., Franze, K. & Steiner, U. Metastable Underwater Superhydrophobicity. Phys. Rev. Lett. 105, 166104 (2010).
Nguyen, T. P. N., Brunet, P., Coffinier, Y. & Boukherroub, R. Quantitative testing of robustness on superomniphobic surfaces by drop impact. Langmuir 26, 18369–18373 (2010).
Bohn, H. F. & Federle, W. Insect aquaplaning: Nepenthes pitcher plants capture prey with the peristome, a fully wettable water-lubricated anisotropic surface. Proc. Natl Acad. Sci. USA 101, 14138–14143 (2004).
Wong, T. S. et al. Bioinspired self-repairing slippery surfaces with pressure-stable omniphobicity. Nature 477, 443–447 (2011).
Epstein, A. K., Wong, T. S., Belisle, R. A., Boggs, E. M. & Aizenberg, J. Liquid-infused structured surfaces with exceptional anti-biofouling performance. Proc. Natl Acad. Sci. USA 109, 13182–13187 (2012).
Kim, P. et al. Liquid-infused nanostructured surfaces with extreme anti-ice and anti-frost performance. ACS Nano 6, 6569–6577 (2012).
Anand, S., Paxson, A. T., Dhiman, R., Smith, J. D. & Varanasi, K. K. Enhanced condensation on lubricant-impregnated nanotextured surfaces. ACS Nano 6, 10122–10129 (2012).
Lafuma, A. & Quere, D. Slippery pre-suffused surfaces. Eur. Phys. J. 96, 56001 (2011).
Ma, W., Higaki, Y., Otsuka, H. & Takahara, A. Perfluoropolyether-infused nano-texture: a versatile approach to omniphobic coatings with low hysteresis and high transparency. Chem. Commun. 49, 597–599 (2013).
Kim, P., Kreder, M. J., Alvarenga, J. & Aizenberg, J. Hierarchical or not? Effect of the length scale and hierarchy of the surface roughness on omniphobicity of lubricant-infused substrates. Nano Lett. 13, 1793–1799 (2013).
Nishiyama, N., Tanaka, S., Egashira, Y., Oku, Y. & Ueyama, K. Vapor-phase synthesis of mesoporous silica thin films. Chem. Mater. 15, 1006–1011 (2003).
Li, Y. et al. Two-dimensional hierarchical porous silica film and its tunable superhydrophobicity. Nanotechnology 17, 238–243 (2006).
Li, Y., Li, C. C., Cho, S. O., Duan, G. T. & Cai, W. P. Silver hierarchical bowl-like array: synthesis, superhydrophobicity, and optical properties. Langmuir 23, 9802–9807 (2007).
He, L. F. et al. Silver nanosheet-coated inverse opal film as a highly active and uniform SERS substrate. J. Mater. Chem. 22, 1370–1374 (2012).
Vogel, N., Weiss, C. K. & Landfester, K. From soft to hard: the generation of functional and complex colloidal monolayers for nanolithography. Soft Matter 8, 4044–4061 (2012).
Shen, X., Ho, C. M. & Wong, T. S. Minimal size of coffee ring sgtructures. J. Phys. Chem. B 114, 5269–5274 (2010).
Wong, T. S., Chen, T. H., Shen, X. & Ho, C. M. Nanochromatography driven by the coffee ring effect. Anal. Chem. 83, 1871–1873 (2011).
Vogel, N., de Viguerie, L., Jonas, U., Weiss, C. K. & Landfester, K. Wafer-scale fabrication of ordered binary colloidal monolayers with adjustable stoichiometries. Adv. Funct. Mater. 21, 3064–3073 (2011).
Vogel, N., Goerres, S., Landfester, K. & Weiss, C. K. A convenient method to produce close- and non-close-packed monolayers using direct assembly at the air-water interface and subsequent plasma-induced size reduction. Macromol. Chem. Phys 212, 1719–1734 (2011).
Li, Y., Lee, E. J. & Cho, S. O. Superhydrophobic coatings on curved surfaces featuring remarkable supporting force. J. Phys. Chem. C 111, 14813–14817 (2007).
Romanov, S. G. et al. Probing guided modes in a monolayer colloidal crystal on a flat metal film. Physical Review B 86, 195145 (2012).
Hall-Stoodley, L., Costerton, J. W. & Stoodley, P. Bacterial biofilms: from the natural environment to infectious diseases. Nat. Rev. Microbiol. 2, 95–108 (2004).
Klevens, R. M. et al. Estimating health care-associated infections and deaths in US hospitals, 2002. Public Health Rep. 122, 160–166 (2007).
Friedlander, R. S. et al. Bacterial flagella explore microscale hummocks and hollows to increase adhesion. Proc. Natl Acad. Sci. USA 110, 5624–5629 (2013).
Meuler, A. J. et al. Relationships between water wettability and ice adhesion. ACS Appl. Mater. Interfaces 2, 3100–3110 (2010).
Wenzel, R. N. Resistance of solid surfaces to wetting by water. Ind. Eng. Chem. 28, 988–994 (1936).
N.V. acknowledges funding from the Leopoldina Fellowship Programme. Wendong Wang and Stefanie Utech are acknowledged for discussions on the modelling of lubricant de-wetting. Jack Alvarenga is acknowledged for help with the ice adhesion setup. The work was supported by the Advanced Research Projects Agency-Energy (ARPA-E) under award number DE-AR0000326 (fabrication and surface properties) and by the Air Force Office of Scientific Research (AFOSR) under award number FA9550-09-0669-DOD35CAP (optical properties). This work was performed in part at the Harvard Center for Nanoscale Systems (CNS) supported by the National Science Foundation (NSF) under award number ECS-0335765.
The authors declare no competing financial interests.
Supplementary Figures S1-S11, Supplementary Tables S1-S4, Supplementary Notes 1-2 and Supplementary Methods (PDF 2946 kb)
Efficient liquid repellency using different lubricants (AVI 11946 kb)
SLIPS-coated watch glass (AVI 6683 kb)
SLIPS-coated and untreated glass vial (AVI 15659 kb)
Adhesion prevention in daily life – an inverse monolayer coated glass slide repels red wine, olive oil and ketchup. (AVI 9814 kb)
Local confinement of water using a coating with locally patterned surface chemistry. (AVI 7306 kb)
Local confinement of octane using a coating with locally patterned surface chemistry. (AVI 6564 kb)
Robustness of lubricated inverse monolayer coatings in daily life applications. (AVI 23489 kb)
About this article
Cite this article
Vogel, N., Belisle, R., Hatton, B. et al. Transparency and damage tolerance of patternable omniphobic lubricated surfaces based on inverse colloidal monolayers. Nat Commun 4, 2176 (2013). https://doi.org/10.1038/ncomms3176
Polymer Journal (2021)
Lubricant-infused directly engraved nano-microstructures for mechanically durable endoscope lens with anti-biofouling and anti-fogging properties
Scientific Reports (2020)
Fabrications and Applications of Slippery Liquid-infused Porous Surfaces Inspired from Nature: A Review
Journal of Bionic Engineering (2019)
Emergent Materials (2019)
Scientific Reports (2017)